Accepted Manuscript The performance of Silver modified Tungsten Oxide for the removal of 2-CP and 2-NP in sunlight exposure: Optical, electrochemical and photocatalytic properties M. Aslam, M. Tahir Soomro, Iqbal M.I. Ismail, N. Salah, M. Waqar Ashraf, Huda A. Qari, A. Hameed PII: DOI: Reference:
S1878-5352(15)00137-9 http://dx.doi.org/10.1016/j.arabjc.2015.05.001 ARABJC 1650
To appear in:
Arabian Journal of Chemistry
Received Date: Accepted Date:
12 January 2015 3 May 2015
Please cite this article as: M. Aslam, M. Tahir Soomro, I.M.I. Ismail, N. Salah, M. Waqar Ashraf, H.A. Qari, A. Hameed, The performance of Silver modified Tungsten Oxide for the removal of 2-CP and 2-NP in sunlight exposure: Optical, electrochemical and photocatalytic properties, Arabian Journal of Chemistry (2015), doi: http:// dx.doi.org/10.1016/j.arabjc.2015.05.001
This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
The performance of Silver modified Tungsten Oxide for the removal of 2-CP and 2-NP in sunlight exposure: Optical, electrochemical and photocatalytic properties M. Aslama, M. Tahir Soomroa, Iqbal M. I. Ismaila,b, N. Salahc, M. Waqar Ashrafd, Huda A. Qarie and A. Hameeda,f* a
Center of Excellence in Environmental Studies (CEES), King Abdulaziz University, Jeddah 21589, Saudi Arabia.
Chemistry Department, Faculty of Science, King Abdulaziz University, Jeddah 21589, Saudi Arabia.
Center of Nanotechnology, King Abdulaziz University, Jeddah 21589, Saudi Arabia.
Department of Mathematics & Natural Sciences, Prince Mohammad Bin Fahd University, Al Khobar 31952, Saudi Arabia.
Biological Department, Faculty of Science, King Abdulaziz University, Jeddah 21589, Saudi Arabia.
National Centre for Physics, Quaid-e-Azam University, Islamabad 44000, Pakistan.
Dr. Abdul Hameed Associate Professor Centre of Excellence in Environmental Studies (CEES) King Abdul Aziz University, Jeddah-21589, Kingdom of Saudi Arabia Contact No: +966-506406684 Email: [email protected]
, [email protected]
Abstract The optical and electrochemical characterization of synthesized Ag+ modified WO3 photocatalysts was performed and its photocatalytic activity was estimated in the visible region (420-800 nm) of sunlight for the degradation of 2-chloro and 2nitrophenol. The catalysts with the varying loading of Ag+ ranging from 0.5% to 10%, exhibited significantly higher activity as compared to pure WO 3. Attempts were made to correlate the enhanced activity of Ag+ loaded catalysts with the optical and electrochemical properties. At lower loading (up to 1% Ag+), the enhanced degradation was attributed to the excited electron trap and transfer ability of surface mounted Ag + species, while the synergic effect between the WO3 support and surface Ag2O resulted the same at higher loadings. The electrochemical properties of the synthesized powders, in comparison to pure WO3, also supported the same findings. The identification of intermediates and estimation of the released anions evidenced the contribution of both hydroxyl radicals (HO•) and superoxide anion (O2•-) radicals in the degradation process. The identification of aliphatic oxygenates as majority intermediates and release of respective ions verified the replacement of Cl- and NO2 groups, insertion of oxygen and aromatic ring cleavage.
Introduction Tungsten oxide (WO3), a photochromic material with a bandgap ranging between
2.4-2.8 eV, being absorptive in the visible region of the solar spectrum, can be a suitable contender for sunlight photocatalytic applications (kominami et al., 2001; Aslam et al., 2014a; Bamwenda and Arakawa, 2001; Zhao et al., 2008). Owing to high recombination rate of charge carriers, a low reduction potential of the excited conduction band electron and low photon conversion efficiency makes WO 3 an inferior choice for environmental applications as compared to ZnO and TiO2 (Tang et al., 2012; Zhao et al., 2012). Various approaches are reported in the literature to address the above-mentioned limitations of photocatalytic materials and augmenting the photocatalytic activity (Rehman et al., 2009; Tang et al., 2013). Among these strategies, surface modifications by metal ion impregnation has proved to be an efficient tool to suppress the charge carrier’s recombination process and improve the activity of a particular photocatalyst (Hameed et al., 2014a; Aslam et al., 2014b; Aslam et al., 2014c; Aslam et al., 2015a; Hameed et al., 2015; Tariq et al., 2015). The mineralization feature of photocatalysis mark it as a promising approach for dealing with environmental decontamination issues (Pichat, 2013). Most of the studies available in the literature for its use in environmental decontamination, particularly for the removal of phenols and its derivatives, are carried in artificial UV or simulated sunlight exposure over either TiO2 or ZnO (Fujishima et al., 2000; Jiuhui, 2008; Bhatkhande et al., 2002; Lettmann et al., 2001; Mills et al., 1993; Chong et al., 2010; Mills and Hunte, 1997; Ollis et al., 1991; Hoffmann et al., 1995; Tang et al., 2011; Tryk et al., 2000; ). Both of these are established active photocatalysts, however, suffer insignificant photon absorption in the visible region of the spectrum that limits their use in the natural sunlight as its major portion (46%) is composed of the visible region. As photocatalysis is entirely dependent on the excitation source, it is now a well-recognized fact that it can only achieve its optimum wide spread efficacy by utilizing economical and renewable excitation source like sunlight (Hameed et al., 2014a; Aslam et al., 2014b; Aslam et al., 2014c; Hameed et al., 2015; Kositzi et al., 2004; Malato et al., 2009; Bahnemann, 2004). Hence the development of sunlight active catalysts, especially 3
capable of utilizing the major portion of the solar spectrum i.e. visible region, is highly desirous. The presence of phenolic compounds mainly chloro and nitro derivatives, due to their health hazards, raises a serious objection on water consumption by living beings. The permissible limits of these derivatives, for human use, is below 1ppm therefore, requires the instant removal (USEPA, 1980). The 2-derivatives of chloro and nitro phenols are the substrates of interest and hard to remove/degrade due to their acute toxicity, high solubility and chemical stability by conventional tools. Additionally the formation of more toxic off shoots during the conventional removal is also unavoidable (Adav et al., 2007; Aslam et al.; 2015b; Calace et al., 2002; Carey, 2000; O’Connor and Young, 1989; Gaya and Abdullah, 2008). Photocatalysis is regarded as a suitable choice for the complete mineralization of pollutants without the formation of secondary pollutants. The current study is an attempt to make WO3 sunlight responsive by using Ag+ as surface modifier to enhance the absorption of photons, suppressing the undesired recombination of charge carriers and improving the photocatalytic activity. The activity of Ag+ modified WO3 was explored in the visible region (420-800 nm) of natural sunlight for the degradation of potential phenolic pollutants like 2-chlorophenol (2-CP) and 2nitrophenol (2-NP). The catalysts used in this work were also utilized in our previous work for the photocatalytic conversion of methane into methanol under the exposure intense 355 nm laser photons (Hameed et al., 2014b). Although the study was useful in explaining various factors involved in the methane conversion process, however, under intense 355 nm laser photons, a number of changes in the catalysts were noticed. The catalysts were re-evaluated by UV-visible diffuse reflectance (DR), photoluminescence (PL) and Raman spectroscopy to explore the possibility for the use in the visible region and their photocatalytic activity was estimated for the removal of 2-CP and 2-NP under mild conditions of sunlight exposure. Additionally, the expediency of the electrochemical tools such as cyclic voltammetry (CV), Electrochemical impedance spectroscopy (EIS) and chronopotentiometry (CP) in predicting the likely photocatalytic behavior of the catalysts, before being subjected to actual photocatalytic experiments, was also estimated.
Synthesis of Ag+ impregnated WO3 Based on the outcomes of previous study, perhaps, the metal loading was not
sufficient enough to furnish any significant change in the activity of 0.1% Ag+ impregnated WO3, for better response in the visible region (420-800 nm) of sunlight, we increased the minimum Ag+ loading from 0.1% to 0.5% in the current study. In the typical synthesis, the required proportions of Ag + ions (0.5%, 1.0%, 5% and 10%) were prepared by dissolving AgNO3 (99.9%) in deionized water and mixed with the appropriate quantity of solid WO3. The slurries were aged overnight at room temperature (24oC) and dried at 150oC under vigorous stirring. The dried powders were subjected to heat treatment at 300oC for the decomposition of nitrates till the complete seizure of NO x. After grinding, the powders were calcined in temperature-controlled furnace at 400oC for 3 h by maintaining the heating rate at 10oC/min (Hameed et al., 2014b).
Characterization of Ag+ impregnated WO3 The solid-state absorption and diffuse reflectance spectra of the synthesized Ag +
impregnated WO3 powders were recorded in the wavelength range of 200-900 nm by Perkin Elmer UV-Visible diffuse reflectance spectrophotometer (DRS) equipped with integrating sphere. The variations in the bandgap with increasing Ag+ loading were evaluated by plotting (F(R) x hυ)1/2 versus hυ (eV), where F(R) is the Kubelka-Munk (KM) transformation of %R values. The photoluminescence (PL) emission spectra of the synthesized Ag+ impregnated powders in comparison to pure WO3, were acquired by a fluorescence spectro-fluorophotometer, RF-5301 PC, Shimadzu, Japan, at an excitation wavelength of 325 nm and slit width of 10 nm. The Raman shifts were measured using a DXR Raman Microscope, Thermo Scientific, USA, equipped with 532 nm laser as the excitation source at 6mW power. Repeated measurements were performed to establish the accuracy and reproducibility of the process.
The X-ray diffraction patterns of the synthesized powders were recorded by a Scintag XDS 2000 diffractometer, equipped with a Cu Kα radiation source in the range of 10 to 90°. The existing phases were identified by matching the acquired XRD patterns with standard JCPDS cards. The XPS profiles of Ag + impregnated powders were acquired by a wide survey scan using X-ray Photoelectron Spectrometer (PHI 5000 VersaProbe II, ULVAC-PHI Inc.). The binding energy was scanned between 0 eV to 1100 eV. The oxidation states of the surface bonded impregnated Ag + ions were evaluated on the basis of the splitting arises due to spin-orbit coupling. The morphology of synthesized powders was evaluated by FESEM (JEOL JSM 6490-A) (Hameed et al., 2014b). A VSP multi-channel potentiostat (Bio-logic Science Instrument, USA) was employed for electrochemical measurements in the dark and under illumination. An electrochemical cell with three-electrode system; glassy carbon electrode (GCE), an Ag/AgCl saturated reference electrode, and a Pt wire counter electrode, was used. For illumination a 50 W halogen lamp was used. All the solutions were prepared in 0.1 M KCl supporting electrolyte, whereas a 2 mM standard solution of ferricyanide was used as redox couple.The chronopotentiometric measurements were carried out in the absence and presence of light by applying a constant current density of 0.05 A/m2 in 0.1 M H2SO4. Electrochemical impedance spectroscopy (EIS) was performed at a bised potential of +0.235 V in 2 mM ferricyanide solution by scannign the frequency from 0.1 Hz to 10 kHz. The EIS Nyquist plots were fitted using Randles electric circuit model by Zfit (Ec-lab software, Bio-logic Science Instruments, USA). For each measurement electrodes were modified with pure and Ag+ impregnated WO3. Prior to modification, glassy carbon electrode was thoroughly cleaned with a diamond and alumina paste manually. The synthesized catalysts were dispersed on the GC electrode by the standard drop coating method. In a typical preparation, the dispersions of pure and Ag+ impregnated WO3 powders were prepared by mixing 1 mg of respective powder in 1 ml of Milli-Q water. The dispersions were homogenized by sonication in an ultrasonic bath for 10 min. For the preparation of thin film electrodes, 20 µL of colloidal suspension was dropped onto the GC electrode and the excess solvent 6
was evaporated by hot air drying. Prior to use in electrochemical measurements, the homogeneity of the film was ensured by optical examination. All the measurements were recorded in comparison to pure WO3. The photocatalytic activity of pure and synthesized Ag+ impregnated WO3 was evaluated in the visible region of sunlight (420-800 nm) for the degradation of 2-CP and 2-NP. Pyrex® glass reactor was utilized as a UV cutoff filter. The dimensions and surface area of the glass reactor was 15.5(diameter) × 2.5(height) and 189 cm2, respectively. In a typical experiment, 200 mg of pure or Ag+ impregnated WO3 was suspended in 150 ml of 50 ppm solution of respective phenol derivatives (2-CP and 2NP). Prior to exposure, to establish equilibrium, the catalyst/phenol suspension was kept in the dark for 1h. Interestingly, the adsorption of both the substrates was significantly low i.e. < 5%. The catalyst/phenol suspension was exposed to the visible region of sunlight and the samples were drawn at regular interval of 30 min in the initial 120 min of exposure and then after every 60 min interval till 240 min. All the experiments were performed under sunlight illumination of 1000±100 × 102 lx during fixed period of sunlight and in the natural environment without stirring. The samples, after removing the catalyst, were analyzed by HPLC (SPD-20A, Shimadzu Corporation, Japan), TOC (Shimadzu Corporation, Japan) and IC (Thermo scientific, USA). For GC-MS analysis the samples collected after 30 min of exposure were extracted thrice with 10 ml of dichloromethane (Sigma-Aldrich, 99.99%) and dried with anhydrous magnesium sulfate for complete removal of water. A GC-MS (Shimadzu Corporation, Japan, ShimadzuQP2010 Plus) equipped with RtX1 capillary column, for the identification of unknown compounds formed as intermediate during the degradation process (Hameed et al., 2014b; Aslam et al., 2014a; Aslam et al., 2014b; Aslam et al., 2014c).
Results and Discussion
Structural and morphological characterization Although, the morphological and structural characterization of the pure
and Ag+ impregnated WO3 by XRD, XPS and FESEM is discussed in detail in our 7
previous communication (Hameed et al., 2014b) however, a brief account is also presented here. It is important to mention here that the additional catalyst synthesized for current work, i.e. 0.5% Ag+ impregnated WO3 was also subjected to the above mentioned characterization, however no significant change in the morphology was observed. The XRD patterns of pure, 1%, 5% and 10% Ag+ impregnated WO3 are compared in Fig. 1. The intense reflections at 2θ values of 23.14o, 23.66o, 24.45o, 33.35o, 34.25o, 41.70o and 44.9o, in all the patterns, were matched with monoclinic WO3 (JCPDS-43-1035). Besides the intense reflections of WO3, additional reflections between 30o and 50o were matched with hexagonal Ag2O (JCPDS-42-0874). For 10% Ag+ loading, the reflection of moderate intensity at 2θ value of 27.5° was matched with Ag2 WO4 (JCPDS-32-1029). This reflection was not noticed for any other Ag+ loaded catalyst. The comparison of the survey scan of pure and 10% Ag + loaded WO3, in the binding energy range of 200 eV to 700 eV, is presented in the Fig. 2a, where the intense peaks due to Ag3d and Ag3p in the binding energy range of 360-380 eV and 550-650 eV, respectively, are noticeable. Additionally, the splitting of the peaks due to spin-orbit coupling is also observable. As presented in Fig.2b, the oxidation states of the Ag species involves were estimated by fitting the splitted Ag3d i.e. Ag3d5/2 and Ag3d3/2 levels. The Ag3d5/2 peak centered at 367.4 eV confirming the existence of impregnated Ag + as surface Ag2O. Additionally, the difference of ~6 eV between the splitted Ag3d 5/2 and Ag3d3/2 levels further confirmed the presence of impregnated Ag+ as Ag2O. The obtained values of 367.4 and 373.5 eV for 3d5/2 and 3d3/2, respectively, were in agreement with the literature values (Hameed et al., 2014b). The FESEM images of the Ag+ loaded WO3, in comparison to pure WO3, are presented in Fig. 3. The Ag+ impregnation resulted no significant change in the morphology of WO3 particles. The FESEM images also verified the presence of Ag + in the form of Ag2O at the surface of WO3 (Hameed et al., 2014b).
Optical characterization The comparison of the solid state absorption spectra of pure and Ag+ impregnated
WO3 recorded between 200 nm to 1000 nm is presented in Fig. 4. Compared to pure 8
WO3, an enhanced absorption in the visible region, due to the increasing surface concentration of Ag+, was noticed for impregnated catalysts. The extent of the absorption for 5% and 10% Ag+ impregnated catalysts with the visual aspect of additional absorption edge was significantly higher than pure WO3 and the impregnated catalysts with a lower concentration of Ag+. The appearance of additional edge is attributed to the formation of Ag2O at the surface. The formation of surface Ag2 O was also endorsed by high resolution FESEM findings (Hameed et al., 2014b), whereas the enhanced absorption in the visible region for the catalysts having lower Ag+ surface loading i.e. 0.5% and 1%, is due to the charge transfer from the O2p levels to the low energy 4d surface states induced by the presence of Ag. The bandgaps of the pure and Ag+ impregnated WO3 catalysts were evaluated by plotting (F(R) x hν) 1/2 versus the photon energy (hν). The F (R) values were estimated by applying Kubelka-Munk transformation of the diffuse reflectance data. This is illustrated in the inset of Fig. 4, presents the comparison of the graphical evaluation of the bandgaps of pure, 1% and 10% Ag+ impregnated WO3. The evaluated bandgap of ~2.7 eV for pure WO3 was in accordance with the literature values (Xu and Schoonen, 2000). A red shift in the band gap of 1% Ag+ impregnated WO3, ~2.5 eV, supports the induction of low energy surface phases by the impregnating Ag+ entities while for 10% Ag+ impregnated WO3, the appearance of absorption edge with the gap of ~2.05 eV depicts the formation of surface Ag2O. The shifting of the bandgap of WO3 base to lower value of ~2.4 eV elaborates the existence of charge transfer synergy. The comparison of the room temperature PL spectra of pure and synthesized Ag + impregnated WO3 is presented in Fig.5a. The appearance of the maxima of the broad emission peak at 467 nm represents the bandgap of WO3 and arises due to the deexcitation from the conduction band (W6+, 4f) to the valence band (O2p) and represents the bandgap excitation. The low intensity peaks at 483 nm and 492 nm signifies the recombination emissions due to the trapping of electrons in the defects generated by the unstable W5+ states created as a result of electron transfer leading to reduction. Compared to pure WO3, a substantial reduction in the luminescence intensity of the abovementioned peaks for Ag+ impregnated catalysts was noticed that depicted the trapping of 9
the excited electrons by the Ag+ induced surface defects thus extended lifetime of the stimulated states. A maximum decrease of ~39% in the emission was noticed for 10% Ag+. The comparison of the Raman spectra of pure and Ag+ impregnated WO3 is presented in Fig. 5b. The characteristic bands of pure WO3 appeared at 271, 326, 716.5
and 806.23 cm-1.The two intense bands at 806.23 and 716.5 cm-1 represents the stretching vibrations O-W-O- while the bands at 271 and 326 cm-1 are due to bending vibrations of W-O-W. The observed values were in accordance with the literature values (Rajagopal et al., 2009; Boulova and Lucazeau, 2002). A marked decrease in the intensity of all peaks, especially the peaks at 806.23 and 716.5 cm-1, for all the Ag+ impregnated catalysts, verified the engagement of singly charged surface oxygen by Ag + forming W-O-Ag type surface entities. The expanded view between 500 cm-1 and 1000 cm-1, as presented in the inset of Fig. 5b, further elaborates the change in the peak intensities with increasing metal loading.
Electrochemical characterization The electrochemical characterization of pure and Ag+ impregnated WO3 powders
was performed by cyclic voltammetry (CV), electrochemical impedance spectroscopy (EIS) and double step chronopotentiometry (CP). Fig.6a shows the comparison of CV curves of pure and Ag+ impregnated WO3 electrodes recorded in 2 mM ferricyanide (K3Fe(CN)6 electrolyte under dark conditions at 50 mV/s between +0.6 V to -0.2 V. The quasi-reversible shapes of CV curves were attributed to the pseudo capacitive behavior of the electrodes. The redox peak pair was assigned to the one electron electrochemical transfer process of Fe3+/Fe2+ couple. The decrease in the current density also verified the successful immobilization of catalysts layers on GCE surface. The non-ideal electrical double layer capacitive behavior exhibited the key role of Ag+ ion on the surface of WO3 as a redox mediator. Under illumination, an enhanced peak current density of the 10% Ag+ impregnated WO3 electrode, compared to that for pure WO3 and other impregnated electrodes, ensured the higher charge transfer ability (Fig. 6b) and attributed to superior conductivity of 10% Ag+ impregnated electrode. The larger specific capacitance or higher conductivity of the Ag+ impregnated photocatalyst was attributed to the formation of surface Ag2O as supported by high resolution FESEM images (Hameed et al., 2014b). 10
The comparison of the EIS spectra of the pure and Ag + impregnated WO3 photocatalysts electrodes in dark is presented in Fig.7a. The utility of the EIS Nyquist plots for the determination of charge resistance and separation efficiency of electron hole pair is established (Lv et al., 2014). Compared to pure WO3, the presence of the large semicircular portions in the EIS Nyquist plots indicated the higher resistances of Ag+ impregnated WO3 to the charge transferand lower conductivity, whereas the reduction of charge transfer resistance of 10% Ag+ impregnated WO3 signifies its higher electrical conductivity (Table1). As presented in Fig. 7b, under illumination, the further decrease in the charge transfer resistance indicated the enhanced conductivity of 10% Ag+ modified electrode surface. As sound agreement was observed between EIS and CV results. The EIS Nyquist plots were fitted using Randles equivalent circuit model and the extracted parameters are presented in Table 1. The charge-discharge behavior and the capability of the synthesized Ag+ impregnated catalysts for capturing or retaining the charge was evaluated by double step chronopotentiometry (CP). The measurements were performed by applying 0.05 A/m2 in in the forward (oxidation) and backward (reduction) direction both in dark and under illumination. The comparison of the galvanostatic charge-discharge cycles, in dark and under illumination, is represented in Fig. 8. The charging curve showed an increase in potential until reaching a plateau, whereas the discharge curve exhibited a sudden drop followed by slow potential decrease. A lower decay rate for 10% Ag+ impregnated WO3 under illumination as compared to other electrodes was witnessed. The unsymmetrical characteristic of charge-discharge curves of different electrodes modified with pure and Ag+ impregnated catalysts showed the absence of electrochemical double layer characteristics rather pseudo capacitive behavior was noticed that implied the excellent capacitive characteristics and electrochemical reversibility. The specific capacitance of the photocatalyst electrodes for discharge was calculated by using the relation below.
Where, Cs (F g–1) is the specific capacitance, I (mA) is discharge current, Δt (s) is the discharge time, ΔV (V) represents the potential drop during discharge, and m (mg) is the mass of the active material loaded on the electrode. The specific capacities of the electrodes for retaining the charge under illumination, evaluated by employing the above relation, were 111.7, 126.6, 127.1, 127.5, and 130.2 (F g–1) for pure, 0.5%, 1%, 5% and 10% Ag+ loaded WO3, respectively. The higher specific capacitance, under illumination, with the increasing Ag+ loading, exhibited the potential of the modified catalysts for capturing and retaining the charge. The findings of CP were also supported by the optical characterization of the Ag+ impregnated catalysts.
Photocatalytic Studies In photocatalysis, the oxidation and reduction sites are generated with the
absorption of photons having energy equal to or higher than the band gap (Eg) of the semiconductor particles. The instantaneous oxidation of the adsorbed H 2O molecules and the reduction of dissolved/adsorbed O2 initiate the generation of a cascade of reactive oxygen species (ROS). Among the ROS identified, hydroxyl radicals and superoxide anions are considered as the primary oxidants that interact and mineralize the contaminants present in the system. The formation of these ions can be represented by the equations below.
H 2 O h H 2 O HO H
(O2 ) adsorbed/ dissolved e O2
The propagation of these species is strongly depending on the potential of the conduction band edge and the pH of the system. The precise role of these ROS in degradation/mineralization of contaminants is not well specified yet, nevertheless, a rough sketch can be drawnon the basis of experimental evidences. 12
The HPLC profiles for the degradation of 2-CP are shown in Fig. S1 (supplementary details). The careful analysis revealed that compared to pure WO3, all the Ag+ loaded catalysts showed noticeably higher activity for the degradation of 2-CP in exposure to the visible region (>420 nm) of natural sunlight. The formation of intermediates revealed the multistep nature of the degradation/mineralization process. The initial formation and gradual decrease in the concentration of intermediates also exposed the simultaneous interaction of ROS with 2-CP substrate and intermediates formed during the photocatalytic process. Initially with the increasing surface density, an increased activity was observed till 1% Ag+ loading, however, a noticeable decrease in the activity was observed for 5% Ag+ loading, whereas a significantly higher activity was witnessed for 10% Ag+ loaded WO3. Although in the lower Ag+ loading range i.e. 1% Ag+ loaded catalyst, the degradation of 2-CP was comparable with that of 10% Ag+ loaded catalyst, however, a marked difference in the removal of intermediates was observed. The intermediate removal efficiency of 10% Ag+ loaded catalyst was distinguishably higher than that of 1% Ag+ loaded catalyst in a visible light exposure. The comparison of the percentage degradation of 2-CP substrate in the visible light exposure to pure and Ag+ loaded WO3 catalysts is presented in Fig. 9a. Compared to ~13% for bare WO3, ~52%, ~39%, ~28% and 56% of 2-CP was degraded in the initial 30 min of exposure of visible light over 0.5%, 1%, 5% and 10% Ag+ impregnated catalysts, respectively. More than 96% removal of 2-CP was observed for 0.5%, 1% and 10% Ag+ loaded WO3 catalysts in 240 min of exposure, whereas ~61% and ~90% of the substrate was removed in the same period of exposure for pure and 5% Ag+ impregnated WO3, respectively. Compared to pure WO3, an overall increase of 40% was estimated for 1% and 10% Ag+ impregnated catalysts. Based on the comparison mentioned above, the higher activity of the Ag+ impregnated catalysts revealed the assistance of surface Ag+ ions in trapping and transfer of photoexcited electrons to the adsorbed species for the generation of ROS. The rate constants ‘k’ of the degradation process was evaluated by applying the Langmuir-Hinshelwood kinetic model. The comparison of the graphical evaluation of the rate constants is presented in Fig. 9b. The calculated rate constants for bare, 0.5%, 1%, 5% and 10% Ag+ impregnated WO3 were 0.0040 min-1, 0.0149 min-1,
0.0141 min-1, 0.0095 min-1 and 0.018 min-1, respectively. The maximum rate of degradation was observed for 10% Ag+ impregnated WO3. The HPLC profiles for the degradation of 2-NP over pure and synthesized Ag+ impregnated WO3 are presented in Fig. S2 (supplementary details). For 2-NP, a trend similar to that of 2-CP degradation, however, a slower rate compared to that of 2-CP was observed. As shown in Fig. 9c, a maximum degradation of ~95% was noticeable for 10%, whereas for 0.5%, 1% and 5% Ag+ impregnated WO3 ~78%, ~85% and ~80% degradation, respectively, was observed. A minimum degradation of ~40% was witnessed for pure WO3. The graphical evaluation of the rate constants for the degradation process is presented in Fig. 9d. The highest rate of degradation of 0.012 min1
was observed for 10% Ag+ modified WO3 while the lowest rate of degradation, 0.0022
min-1 was noticed for pure WO3. For 0.5%, 1% and 5% Ag+ modified WO3, the rate constants with the minor difference i.e. 0.0062 min-1, 0.0074 min-1 and 0.0066 min-1, respectively, were observable. The mineralization efficiency of bare and Ag+ modified WO3 catalysts in terms of TOC removal as a function of sunlight (>420 nm) exposure time is presented in Fig. 10a. Compared to the degradation, a significantly lower mineralization especially in the initial 90 min of the exposure was observed and the maximum TOC removal of >90% was observed for 10% Ag+ impregnated WO3. A TOC removal of ~59%, ~89%, and ~69% were observed for 0.5%, 1% and 5% Ag+ impregnated WO3, respectively, in 240 min of sunlight (>420 nm) was noticed. The minimum TOC removal of ~40% was observed for pure WO3. An increase in the mineralization was noticed with the decrease in the concentration of the 2-CP substrate with time, however, a trend similar to that of degradation process was observed in the removal of total organic carbon. As presented in Fig. 10b, the graphical evaluation of rate constants for the TOC removal of 2-CP, similar to degradation process, Langmuir-Hinshelwood kinetic model also holds good for TOC removal with reasonable correlation. The calculated rate constants of TOC removal for pure, 0.5%, 1%, 5% and 10% Ag+ impregnated WO3 were 0.0025 min-1, 0.0040 min-1, 0.0097 min-1, 0.0054 min-1 and 0.012 min-1, respectively.
As presented in Fig. 10c, a similar situation was perceived in the mineralization of 2-NP. The 10% Ag+ impregnated WO3 was found most active that efficiently removed 84% of TOC in 4 h of sunlight (> 420 nm) exposure. The activities of 0.5% and 1% Ag+ loaded catalysts (60% and 66% TOC removal, respectively) were compared with each other, but significantly lower than 10% Ag+ loaded and higher than pure WO3. Among the impregnated catalysts, the minimum TOC removal i.e. ~50% was observed for 5% Ag+ impregnated WO3. The rate constants of the TOC removal (Fig. 10d) were 0.0015 min-1, 0.0041 min-1, 0.0046 min-1, 0.0030 min-1 and 0.0078 min-1 for pure, 0.5%, 1%, 5% and 10% Ag+ loaded WO3, respectively. The enhanced degradation by Ag+ impregnated catalysts, compared to WO3 clearly revealed that the presence of Ag+ at the surface not only notably suppresses the undesired electron hole pair recombination but promotes the efficient electron transfer to adsorbed/dissolved species for the generation of reactive oxygen species. The suppression of the recombination process was also evidenced in the PL analysis (Fig. 5a). Additionally, the decreased impedance (Fig. 7) and slow discharge (Fig. 8) of the impregnated catalysts compared to pure WO3 elaborated the increased conductivity and enhanced capacity for the retention of charge which is a required phenomenon in photocatalytic processes. In the current study, the majority role of the ROS either superoxide anion (O2•−) or hydroxyl radicals (HO•) was assessed on the basis of the identification of intermediates by analyzing the samples drawn after 30 min of sunlight (>420 nm) using GC-MS for 1% and 10% Ag+ impregnated WO3 catalysts both for 2-CP and 2-NP. The presence of substrate in GC-MS analysis was used as a marker. The major findings of the analysis were as follows:
Majority intermediates were aliphatic oxygenates that included C1-C8 alcohols, esters and carboxylic acids.
Hydroxyl group substituted phenols were also identified in smaller fraction for 1% Ag+ impregnated catalyst and in appreciable concentration for 10% Ag+ impregnated WO3.
A number of common products such as CH3COOH, CH3COOCH3 etc. were also identified for both 2-CP and 2-NP.
Coupling products were also identified for phenolic substrate.
The findings of GC-MS analysis revealed superoxide radicals as the leading facilitators in the degradation and mineralization process. Additionally the intermediates formed by the interaction of hydroxyl radicals with the phenolic substrates (2-CP and 2NP) are further interacted by the superoxide anions to aliphatic oxygenates initially and to mineralization finally. The rapid TOC removal also supports the similar conclusion. The potential of valence (+3.44 V) and conduction (+0.74 V) band edge of WO3 demonstrates its disability for the reduction of dissolved/adsorbed O 2 while the suitability for the oxidation of water and thus the formation of hydroxyl radicals. In our previous communication (Aslam et al., 2014a), we proposed the plausible mechanism for the generation of superoxide anion radicals for pure WO3, however, due to the surface presence of Ag+, the applicability of the proposed mechanism is questionable. On the other hand, the formation of aliphatic oxygenates in the system,as identified by the GCMS analysis, stress the existence of superoxide radicals in majority. This situation leads to the presumption that the surface Ag+ species play a very vital role in the trapping and transfer of excited electrons. To sketch the possible mechanism of electron trapping and transfer, it may be presumed that the photo-excited electrons (e-) are directly transferred to the Ag+ species as in the form of surface Ag2O, as verified by XPS and XRD analysis, that are transiently converted to Ago•AgO couple. After transferring the captured electrons to the dissolved/adsorbed O2, Ago•AgO is transformed back to Ag2O instantaneously. The valence band entrapped photogenerated holes (h+) oxidize the adsorbed water for the generation of hydroxyl radicals. This mechanism seems rational for lower concentrations i.e. 0.5% and 1% Ag+ impregnated catalysts, as the impregnated Ag+ ions form surface bound Ag2O by sharing the surface oxygen thus sharing the valence band of WO3. The above mentioned mechanism is given in scheme I below. Scheme I
Ag 2O @WO3 h Ag 2O @WO3 (h , e ) Ag AgO @WO3 (h ) Ag AgO @WO3 ( h ) O2 H 2 O Ag 2 O @WO3 O2 HO H
The decrease in the pH of the system during the course of the photocatalysis process also supports the above described mechanism. At higher concentrations i.e. 5% and 10% Ag+ impregnated WO3, with the increase in the surface density, along with the prevalent mechanism stated above, a reasonable fraction of photons is directly absorbed by Ag2O particles that enhances the production of both superoxide anion (O2•−) or hydroxyl radicals (HO•). Additionally, the suitability of the potentials of valence and conduction band edges of both Ag2O and WO3 promotes the mutual transfer of charge carriers among the two and enhances the lifetime of the excited states. These transitions, as mentioned in the scheme II below, leads to enhanced the generation of hydroxyl radicals, however, based on energy consolations cannot affect the formation of superoxide anion (O2•−) radicals. The generation of superoxide anion (O2•−) radicals, in the current system, is possible by the mechanism postulated above. The enhanced yield of OH substituted intermediates, as identified by GC-MS, support the enhanced yield of hydroxyl radicals at higher Ag+ loadings. Scheme II
Ag 2 O @WO3 h Ag 2 O @WO3 ( h ,e ) Ag 2 O( h ) @WO3 ( e )
Ag 2 O @WO3 h Ag 2 O( h ,e ) @WO3 Ag 2 O( h ) @WO3 ( e )
Fig. S3 (supplementary details) shows the IC profile of the released anions during the course of degradation process for 2-CP and 2-NP over 10% Ag+ impregnated WO3. It was observed that the concentration of Cl- ions in the solution increases with the increase 17
in sunlight (>420 nm) exposure time during 2-CP degradation, whereas for 2-NP, a major peak of NO3 - ions were identified in the solution instead of NO2 - ions. The release of ions in the degradation of phenolic substrates and identification of aliphatic oxygenates as intermediates lead to the conclusion that the bulk of 2-CP and 2-NP are degraded by the interaction of charged rather than neutral ROS. Also the ROS mainly, i.e. superoxide anion radicals (O2•−) are incorporated in the structure by displacing the Cl- or NO2- ions and ripping apart the aromatic system. The released ions and the intermediates formed are further interacted by the superoxide anion radicals (O2•−) leading to further oxidation. The presence of C1-C4 oxygenates among the intermediates formed further strengthens the view that after initial degradation the mineralization proceeds by fragmentation. The fragments are interacted by the superoxide anion radicals till complete mineralization. The graphical comparison of the released ions during the degradation of 2-CP is presented in Fig. 11a. It was observed that a minor fraction of released Cl- ions are further oxidized to ClO2 -, ClO3 - and ClO4- ions. Noticeably, the majority of the released chloride ions remains in the solution without further interaction with ROS. On the other hand, as presented in Fig. 11b, for 2-NP, surprisingly, a very small fraction of NO2 - ions were detected in the solution for this particular system. This observation led to the reasoning that all the released NO2- ions are immediately transformed to NO3- ions. To further explore the possible reasons and mechanism of instantaneous conversion of NO2 - ions to NO3- ions, the pH changes of the system were monitored. For 10% Ag + impregnated WO3 the initial pH recorded in the dark with 2-NP substrate was 5.4 which fall to 5 in the initial 30 min of sunlight (>420 nm). The pH of the system gradually decreased with the increase in exposure time, however, did not exceed the pH value of 4.6 till the completion of the experiment in 240 min. Under similar conditions, for 2-CP, the pH decreased to 4.4. For 2-NP, among all the catalysts, including pure WO3, the pH of pure and 0.5% Ag+ impregnated WO3 reached the neutral pH value of 7 in the above mentioned period. The observed pattern of pH change for pure WO3 was similar to that already reported (Aslam et al., 2014a) with minor deviation that may be due to the changed morphology and elimination of UV region of sunlight. Keeping in view the pH changes of the system, the following mechanism has been postulated for the instantaneous transformation of NO 2 - to NO3- ions. 18
NO2 H HNO2 HNO2 O2 NO3 HO
The proposed mechanism is not only supported by the pH changes during the course of degradation in visible light but also by the enhanced formation of HO • substituted products as intermediates because of the enhanced yield of hydroxyl radicals.
Conclusions The surface presence of Ag+ improves both the optical and electrochemical
properties of WO3 and makes it responsive and active in the visible region of sunlight. The study demonstrated that the electrochemical characterization in the dark as well as under illumination furnishes vital information regarding the expected behavior of the photocatalytic material. The silver ions after being converted to Ag2O under calcination facilitates the trapping and transfer of the photo-excited electrons that lead to enhanced generation of reactive oxygen species in the system thus enhancing the degradation as well as mineralization process. The presence of chloro and nitro group in the phenol assists in the degradation process by providing the sites of interaction for the incoming ROS. Both the intermediates and substrates are treated simultaneously that leads to complete mineralization. The released ions are subjected to further oxidation. The study provides a base for the development of visible light active photocatalysts for water decontamination.
Acknowledgements We acknowledge the support from Center of Excellence in Environmental Studies (CEES), King Abdulaziz University and Ministry of Higher Education (MoHE) of Saudi Arabia.
References Adav, S.S., Chen, M.Y., Lee, D.J., Ren, N.Q., 2007. Chemosphere 67, 1566– 1572. Aslam, M., Ismail, I.M.I., Chandrasekaran, S., Hameed, A., 2014a. J. Hazard. Mater. 276, 120-128. Aslam, M., Ismail, I.M.I., Chandrasekaran, Almeelbi, T., Hameed, A., 2014b. RSC Adv., 4, 49347-49359. Aslam, M., Ismail, I.M.I., Almeelbi, T., Salah, N., Chandrasekaran, S., Hameed, A., 2014c. Chemosphere 117C, 115-123. Aslam, M., Ismail, I.M.I., Chandrasekaran, S., Salah, N., Qari, H.A., Hameed, A., 2015a. Water Air Soil Pollut. 226, 70. Aslam, M., Ismail, I.M.I., Salah, N., Chandrasekaran, S., Qamar, M.T., Hameed, A., 2015b. J. Hazard. Mater. 286, 127–135. Bahnemann, D., 2004. Sol. Energy 77, 445–459. Bamwenda, G.R., Arakawa, H., 2001. App. Catal. A: Gen. 210, 181-191. Bhatkhande, D.S., Pangarkar, V.G., Beenackers, A.A.C.M., 2002.
J. Chem. Tech.
Biotech. 77, 102–116. Boulova, M., Lucazeau, G., 2002. J. Solid State Chem. 167, 425-434. Calace, N., Nardi, E., Petronio, B.M., Pietroletti, M., 2002. Environ. Pollut. 118, 315319. Carey, F.A., 2000. OrganicChemistry, fourthed. McGraw-Hill, New York. p. 945. Chong, M.N., Jin, B., Chow, C.W.K., Saint, C., 2010. Water Res.44, 2997–3027. Fujishima, A., Rao, T.N., Tryk, D.A., 2000. J. Photochem. Photobiol. C: Photochem. Rev. 1, 1–21. Gaya, U.I., Abdullah, A.H., 2008. J. Photochem. Photobiol. C Photochem. Rev. 9, 1–12. Hoffmann, M.R., Martin, S., Choi, W., Bahnemann, D.W., 1995. Chem. Rev. 95, 69–96. Hameed, A., Aslam, M., Ismail, I.M.I., Chandrasekaran, S., Kadi, M.W., Gondal, M.A., 2014a. Appl. Catal., B 160-161, 227-239. Hameed, M., Ismail, I.M.I., A., Aslam, Gondal, M.A., 2014b. Appl. Catal. A: Gen. 470, 327-335.
Hameed, A., Aslam, M., Ismail, I.M.I., Salah, N., Fornasiero, P., 2015. Appl.Catal. B: Environ. 163, 444-451. Jiuhui, Q.U., 2008. J. Environ. Sci. 20, 1-13. Kominami, H., Yabutani, K.I., Yamamoto, T., Kera, Y., Ohtani, B., 2001. J. Mater. Chem. 11, 3222-3227. Kositzi, M., Poulios, I., Malato, S., Caceres, J., Campos, A., 2004. Water Res. 38, 11471154. Lettmann, C., Hinrichs, H., Maier, W.F., 2001. Angew. Chem. Int. Ed. 40, 3160–3164. Lv, H., Liu, Y., Hu, J., Li, Z., Lu, Y., 2014. RSC Adv., 4, 63238-63245 Malato, S., Fernández-Ibáñez, P., Maldonado, M.I., Blanco, J., Gernjak, W., 2009. Catal. Today 147, 1–59. Mills, A., Davies, R.H., Worsley, D., 1993. Chem. Soc. Rev. 22, 417-425. Mills, A., Le Hunte, S., 1997. J. Photochem. Photobiol., A 108, 1–35. O'Connor, O.A., Young, L.Y., 1989. Environ. Toxicol. Chem. 8, 853-862. Ollis, D.F., Pelizzetti, E., Serpone, N., 1991. Environ. Sci. Technol. 25, 1522–1529. Pichat, P., 2013. Photocatalysis and Water Puriﬁcation: From Fundamentals to Recent Applications, ﬁrst ed. Wiley-VCH Verlag, Weinheim, Germany. Qamar, M.T., Aslam, M., Ismail, I.M.I., Salah, N., Hameed, A., 2015. ACS Appl. Mater. Interfaces. DOI: 10.1021/acsami.5b01273. Rajagopal, S., Nataraj, D.,Mangalaraj, D.,Djaoued, Y., Robichaud, J., Khyzhun, O.Y., 2009.Nanoscale Res. Lett. 4, 1335-1342. Rehman, S., Ullah, R., Butt, A.M., Gohar, N.D., 2009. Strategies of making TiO2 and ZnO visible light active. J. Hazard. Mater. 170, 560-569. Tang, Y., Subramaniam, V.P., Lau, T.H., Lai, Y., Gong, D., Kanhere, P.D., Cheng, Y.H., Chen, Z., Dong, Z., 2011. Appl. Catal., B 106, 577–585. Tang, Y., Wee, P. Lai, Y., Wang, X., Gong, D., Kanhere, P.D., Lim, T.T., Dong, Z., Chen, Z., 2012. J. Phys. Chem. C 116, 2772−2780. Tang, Y., Jiang, Z., Xing, G., Li, A., Kanhere, P.D., Zhang, Y., Sum, T.C., Li, S., Chen, X., Dong, Z., Chen, Z., 2013. Adv. Funct. Mater. 23, 2932–2940. Tryk, D.A., Fujishima, A., Honda, K., 2000. Electrochim. Acta 45, 2363–2376.
U.S. Environmental Protection Agency, 1980. Ambient Water Quality Criteria for Nitrophenols, Washington, DC. Xu, Y., Schoonen, M.A.A., 2000. Am. Mineral. 85, 543-556. Zhao, Z.G., Miyauchi, M., 2008. Angew. Chem. Int. Ed. 47, 7051-7055. Zhao, W., Wang, Z., Shen, X., Li, J., Xu, C., Gan, Z., 2012. Int. J. Hydrogen Energy. 37, 908-15.
The comparison of XRD patterens of pure, 1%, 5% and 10% Ag+ impregnated WO3. The arrows indicate the growth of reflections arising Ag 2O (Hameed et al., 2014b).
(a) The comparison of the survey scan of pure and 10% Ag+ impregnated WO3 in the binding energy range of 200 to 700 eV. The peaks arising due to Ag3d and Ag3p are marked. (b) The fitted Ag 3d splitted levels in 10% Ag + impregnated WO3 (Hameed et al., 2014b).
The FESEM high resolution images (× 250,000) of pure and Ag+ modified WO3. (Hameed et al., 2014b).
(a) The comparison of the solid-state absorption spectra of pure and Ag+ modified WO3. The inset shows the graphical evaluation of the bandgap of pure, 1% and 10% Ag+ impregnated WO3.
(a) The comparison of the photoluminescence (PL) spectra of pure and Ag+ modified WO3. The samples were excited at a wavelength of 325 nm and the emissions were recorded from 350 to 850 nm. (b) The comparison of the effect 27
of Raman shift of WO3 with the increasing Ag+ loading. The inset shows the Raman shift between 500 to 1000 nm.
Fig. 6. The comparison of the cyclic voltammetric behaviour of pure and Ag+ modified WO3 (a) in dark (b) under illumination in 2 mM solution of Fe3+/ Fe2+ as redox couple using GC electrode. 29
Fig. 7. The comparison of the EIS Nyquist plots of pure and Ag+ modified WO3 (a) in dark (b) under illumination in 2 mM solution of Fe3+/ Fe2+ as redox couple using GC electrode. The insets of (a) and (b) shows the exploded view of the semicircular regions of the plots. 30
Fig. 8. The two-step Chronopotentiometric curves of pure and Ag+ modified WO3 electrodes in (a) dark (b) under illumination during constant current density in 2 mM solution of Fe3+/ Fe2+ as redox couple using GC electrode.
The comparison of the percentage degradation of (a) 2-CP (b) the graphical evaluation of rate constant “k” for the degradation of 2-CP (c) the percentage degradation of 2-NP (d) the graphical evaluation of rate constant “k” for the degradation of 2-NP in the presence of pure and Ag+ modified WO3 in the exposure of visible portion (> 420 nm) of natural sunlight.
Fig. 10. The comparison of the percentage TOC removal of (a) 2-CP (50 ppm) (b) 2-NP (50 ppm) in the presence of pure and Ag+ modified WO3 in the exposure of visible portion (> 420 nm) of natural sunlight Whereas (c) and (d) shows the graphical evaluation of rate constants for 2-CP and 2-NP, respectively.
Fig. 11. The graphical comparison for the release as well as conversion of ions during the degradation of (a) 2-CP and (b) 2-NP (50 ppm each).
Table 1: The parameters extracted from the fitted EIS Nyquist plot for pure and Ag+ modified WO3 in dark and under illumination. Catalysts
Dark Rs (Ohm)
Wz (Ohm / s1/2)
0.5% [email protected]
1% Ag @ WO3
5% [email protected]
10% [email protected]
0.5% [email protected]
1% [email protected]
5% [email protected]
10% Ag @ WO3
Under illumination 19.62